Survey

* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

Document related concepts

Grow light wikipedia , lookup

Architectural lighting design wikipedia , lookup

Phosphor wikipedia , lookup

Daylighting wikipedia , lookup

Photon wikipedia , lookup

Bioluminescence wikipedia , lookup

Doctor Light (Kimiyo Hoshi) wikipedia , lookup

Doctor Light (Arthur Light) wikipedia , lookup

Photopolymer wikipedia , lookup

Photoelectric effect wikipedia , lookup

Transcript
```Dr. Ali Abadi
Chapter Eight: Optical Properties
Materials Properties
Light is an electromagnetic wave or photon. In the classical sense, electromagnetic radiation is
considered to be wave-like, consisting of electric and magnetic field components that are
perpendicular to each other and also to the direction of propagation as shown in figure below.
The velocity of light is c = 3 x 108m/sc
The spectrum consists of radiation such as gamma rays, x-rays, ultraviolet, visible, infrared and
radio. Visible light lies within a very narrow region of the spectrum, with wavelengths ranging
between about 0.4µm (4x10-7 m) for violet and 0.7µm for red color.
All electromagnetic radiation traverses a vacuum at the same velocity, that of lightβnamely, 3 x 108
m/s (186,000 miles/s). This velocity, c, is related to the electric permittivity of a vacuum and the
magnetic permeability of a vacuum through
π=
1
π0 π0
π
Energy of photon is πΈ = βπ = βπ = β π
h: Planckβs constant = 6.63x10-34J-s
1
f = π is a frequency (Hz)
c is the speed of light = 3x108 m/s
π is a wave length (m)
Example: Visible light having a wavelength of 5 x10-7 m appears green. Compute the frequency and
energy of a photon of this light.
We must compute the frequency of a photon of green light,
Ξ½ =cΞ»=3x108m/s . 5x10β7m= 6 x 1014 s-1 (Hz)
The energy a photon of green light
E =hc / Ξ»=(6.63x10β34J-s)(3x108m/s) / 5x10β7m
= 3.98 x 10-19 J = (2.48 eV)
Light Interactions With Solids:
When light proceeds from one medium into another (e.g., from air into a solid substance), several
things happen. Some of the light radiation may be transmitted through the medium, some will be
absorbed, and some will be reflected at the interface between the two media. The intensity IO of the
beam incident to the surface of the solid medium must equal the sum of the intensities of the
transmitted, absorbed, and reflected beams, denoted as IT, IA, and IR respectively, or
IO = IT + IA + IR
T = IT /I0
A = IA /I0
R = IR /I0
T~1 :
T~0 :
Transmissivity
Absorptivity
Reflectivity
Transparent
Opaque
T+A+R=1
Example: Distinguish between materials that are opaque, translucent, and transparent in terms of
their appearance and light transmittance
.
Opaque materials are impervious to light transmission; it is not possible to see through them.
Light is transmitted diffusely through translucent materials (there is some internal light scattering).
Objects are not clearly distinguishable when viewed through a translucent material.
Virtually all of the incident light is transmitted through transparent materials, and one can see clearly
through them.
2
In figure above three (3) things can happen.
ο·
ο·
ο·
Light passes through easily (if the object is transparent) βMaterial is capable of
transmitting light with little absorption or reflection β O n e c a n s e e t h r o u g h
them
Light is blurred (if the object is translucent) βMaterials through which light is
transmitted diffusely β L i g h t i s s c a t t e r e d w i t h i n t h e m a t e r i a l β O b j e c t s a r e
not clearly visible through the material
Light is blocked (if the object is opaque) βMaterials which are impervious to the
transmission of visiblelight
Atomic And Electronic Interactions:
ο·
The optical phenomena that occur within solid materials involve interactions between the
electromagnetic radiation and atoms, ions, and/or electrons.
ο· Two of the most important of these interactions are electronic polarization and electron
energy transitions.
Electronic Polarization:
ο·
ο·
ο·
One component of an electromagnetic wave is simply a rapidly fluctuating electric field.
For the visible range of frequencies, this electric field interacts with the electron cloud
surrounding each atom within its path in such a way as to induce electronic polarization, or to
shift the electron cloud relative to the nucleus of the atom with each change in direction of
electric field component.
Two consequences of this polarization are: (1) some of the radiation energy may be absorbed,
and (2) light waves are retarded in velocity as they pass through the medium.
3
Electron Transitions:
The absorption and emission of electromagnetic radiation may involve electron transitions from one
energy state to another.
When a photon, or packet of light energy, is absorbed by an atom, the atom gains the energy of the
photon, and one of the atom's electrons may jump to a higher energy level. The atom is then said to
be excited. When an electron of an excited atom falls to a lower energy level, the atom may emit the
electron's excess energy in the form of a photon. The energy levels, or orbitals, of the atoms shown
here have been greatly simplified to illustrate these absorption and emission processes. For a more
accurate depiction of electron orbitals, see Atom and Atomic Theory.
ΞπΈ = βπ
Optical Properties of Metals:
ο·
ο·
ο·
ο·
ο·
ο·
ο·
ο·
Metals are opaque because the incident radiation having frequencies within the visible range
excites electrons into unoccupied energy states above the Fermi energy, as demonstrated in
Figure (a) below.
Total absorption is within a very thin outer layer, usually less than 0.1 µm thus only metallic
films thinner than 0.1 µm are capable of transmitting visible light.
In fact, metals are opaque to all electromagnetic radiation on the low end of the frequency
spectrum, from radio waves, through infrared, the visible, and into about the middle of the
Metals are transparent to high-frequency (x- and Ξ³-ray) radiation.
All frequencies of visible light are absorbed by metals because of the continuously available
empty electron states, which permit electron transitions.
Most of the absorbed radiation is reemitted from the surface in the form of visible light of the
same wavelength, which appears as reflected light.
Aluminum and silver are two metals that exhibit this reflective behavior.
Copper and gold appear red-orange and yellow, respectively, because some of the energy
associated with light photons having short wavelengths is not reemitted as visible light.
4
Typical band structures:
Example: Briefly explain why metals are opaque to electromagnetic radiation having photon
energies within the visible region of the spectrum.
The electron band structures of metals are such that empty and available electron states are adjacent
to filled states. Electron excitations from filled to empty states are possible with the absorption of
electromagnetic radiation having frequencies within the visible spectrum. The light energy is totally
absorbed or reflected, and, since none is transmitted, the material is opaque.
5
Optical Properties of metals:
ο·
ο·
ο·
All frequencies of visible light are absorbed by metals because of the continuously available
empty electron states, which permit electron transitions.
Metals are opaque to all electromagnetic radiation on the low end of the frequency spectrum,
from radio waves, through infrared, the visible, and into about the middle of the ultraviolet
Most of the absorbed radiation is reemitted from the surface in the form of visible light of the
same wavelength, which appears as reflected light; an electron transition accompanying
Refraction :
Light that is transmitted into the interior of
transparent materials experiences decrease in
velocity and as result is bent at the interface; this
phenomenon is termed refraction. The index of
refraction n of a material is defined as the ratio of
the velocity in vacuum c to the velocity in the
medium Ξ½ , or
The magnitude of n (or the degree of
bending) will depend on the wavelength of
the light. This effect is graphically
demonstrated by the familiar dispersion or
separation of a beam of white light into its
component colors by a glass prism.
6
Each color is deflected by a different amount as it passes into and out of the glass, which results in the separation of
colors.
If the angle of incidence from a normal to the surface is ΞΈ , and the angle of refraction is ΞΈ , the
i
r
refractive index of the medium, n, is given by (provided that the incident light is coming from a
phase of low refractive index such as vacuum or air) π =
ο·
sin π π
sin ππ
speed of light in a material can
be related to its electrical and magnetic
properties as
π=
1
ππ
where Ξ΅ β electrical permittivity, and ΞΌ β
magnetic permeability. Thus,
π=
π
=
π
ππ
π 0 π0
=
ππ ππ
Since most materials are only slightly magnetic i.e. ΞΌ β1, Thus
r
π=
ππ
Snellβs law of light refraction: refractive indices for light passing through from one medium with
refractive index n through another of refractive index nβ is related to the incident angle, ΞΈ, and
refractive angle, ΞΈβ, by
π
sin π β²
=
πβ²
π πππ
Example: Compute the velocity of light in diamond, which has a dielectric constant ππ of 5.5 (at
frequencies within the visible range) and a magnetic susceptibility of -2.17 x 10-5.
ο
Ξ΅ = Ξ΅rΞ΅0 = (5.5)(8.85 x 10-12 F/m) = 4.87 x 10-11 F/m
ΞΌ = ΞΌ0ΞΌr=ΞΌ0(Οm + 1) = (1.257 x 10-6 H/m)(1 β 2.17 x 10-5) = 1.257 x 10-6 H/m
π=
1
ππ
= 1 / {(4.87x10β11F/m)(1.257x10β6H/m)}0.5
=1.28 x 108m/s
Reflection :
When light radiation passes from one medium into another having a different index of refraction,
some of the light is scattered at the interface between the two media even if both are transparent. The
reflectivity R represents the fraction of the incident light that is reflected at the interface, or
7
where I0 and IR are the incident and reflected beams intensities respectively. If the light is
normal (or perpendicular) to the interface, then
where and are the indices of refraction of the two media. If the incident light is not normal to the
interface, R will depend on the angle of incidence. When light is transmitted from a vacuum or air
into a solid s, then
Example: It is desired that the reflectivity of light at normal incidence to the surface of a transparent
medium be less than 5.0%.Which of the following materials: sodaβlime glass, Pyrex glass, periclase,
spinel, polystyrene, and polypropylene? Justify your selections.
0.050 = (nsβ1)2 / (ns+1)2= (ns2β2ns+1) / (ns2+2ns+1)
or, upon rearrangement 0.95ns2 β 2.10ns + 0.95 = 0
The value of ns is determined by using the quadratic equation solution as follows:
ns=β(β2.10)±{(β2.10)2β(4)(0.95)(0.95)}0.5 / (2)(0.95) = (2.10±0.894) / 1.90
The two solutions are: ns(+) = 1.576 and ns(β) = 0.634.
The ns(+) solution is the one that is physically reasonable. Thus, of the materials listed in tables,
soda-lime glass, Pyrex glass, and polypropylene have indices of refraction less than 1.576, and would
be suitable for this application.
Example: The index of refraction of quartz is anisotropic. Suppose that visible light is passing from
one grain to another of different crystallographic orientation and at normal incidence to the grain
boundary. Calculate the reflectivity at the boundary if the indices of refraction for the two grains
are 1.544 and 1.553 in the direction of light propagation.
R = (n2βn1)2 / (n2+n1)2
= (1.553β1.544)2 / (1.553+1.544)2= 8.45 x 10-6
Absorption :
ο·
ο·
ο·
ο·
Nonmetallic materials may be opaque or transparent to visible light; and, if transparent they
often appear colored. In principle, light radiation is absorbed in this group of materials by
two basic mechanisms, which also influence the transmission characteristics of these
nonmetals.
One of these is electronic polarization. Absorption by electronic polarization is important
only at light frequencies in the vicinity of the relaxation frequency of the constituent atoms.
The other mechanism involves valence band-conduction band electron transitions, which
depend on the electron energy band structure of the material.
Absorption of a photon of light may occur by the promotion or excitation of an electron from
the nearly filled valence band, across the band gap, and into an empty state within the
conduction band.
8
ο·
Every nonmetallic material becomes opaque at some wavelength, which depends on the
magnitude of its Eg. For example, diamond, having a band gap of 5.6 eV, is opaque to
Eg (min)=hc/Ξ»(max)=1.8 eV (Ξ»=700 nm)
Eg< 1.8 eV, all visible light is absorbed
1.8 eV< Eg< 3.1 eV, Colored
Eg>3.1 eV, transparent to visible light
ο·
ο·
ο·
ο·
When a light beam in impinged on a material surface, portion of the incident beam that is not
reflected by the material is either absorbed or transmitted through the material.
Bouguerβs law: The fraction of beam that is absorbed is related to the thickness of the
materials and the manner in which the photons interact with the materialβs structure.
π°β²π» = π°β²π πβπ·π
where Iβ β intensity of the beam coming out of the material,
Iβ β intensity of the incident beam,
ο·
ο·
x β path through which the photons move, and
π·β linear absorption coefficient in (mm-1), which is characteristic of a particular material.
ο·
0
Absorption mechanisms
ο·
ο·
ο·
ο·
ο·
Absorption occurs by two mechanisms: Rayleigh scattering and Compton scattering.
Rayleigh scattering: where photon interacts with the electrons orbiting an atom and is
deflected without any change in photon energy. This is significant for high atomic number
atoms and low photon energies. Ex.: Blue color in the sunlight gets scattered more than other
colors in the visible spectrum and thus making sky look blue.
Tyndall effect is where scattering occurs from particles much larger than the wavelength of
light. Ex.: Clouds look white.
Compton scattering: interacting photon knocks out an electron loosing some of its energy
during the process. This is also significant for high atomic number atoms and low photon
energies.
Photoelectric effect occurs when photon energy is consumed to release an electron from
atom nucleus. This effect arises from the fact that the potential energy barrier for electrons is
finite at the surface of the metal. Ex.: Solar cells.
9
Example: Zinc selenide (ZnSe) has a band gap of 2.58 eV. Over what range of wavelengths of
visible light is it transparent?
Only photons having energies of 2.58 eV or greater are absorbed by valence-band-to-conductionband electron transitions. The minimum photon energy for visible light is 1.8 eV, which corresponds
to a wavelength of 0.7 ΞΌm.
ο
Ξ» = hc / E= (4.13x10β15eV-s)(3x108m/s) / 2.58eV = 4.80 x 10-7 m = 0.48 ΞΌm
Thus, pure ZnSe is transparent to visible light having wavelengths between 0.48 and 0.7 ΞΌm.
Example: The fraction of nonreflected radiation that is transmitted through a 5-mm thickness of a
transparent material is 0.95. If the thickness is increased to 12 mm, what fraction of light will be
transmitted?
π°β²π» = π°β²π πβπ·π ,
ln (IT' / I0') = β Ξ²x
ο
Ξ² =(β1 / x) ln IT' / I0' = β (15mm) ln(0.95) = 1.026 x 10-2 mm-1
And computation of IT'/I0' when x = 12 mm , IT' / I0'= exp (β Ξ²x)
=exp[β(1.026x10β2mmβ1)(12mm)]= 0.884
Transmission :
The phenomena of absorption, reflection, and transmission may be applied to the
passage of light through a transparent solid.
For an incident beam of intensity I0 that impinges on the front surface of a specimen of thickness l
and absorption coefficient ß the transmitted intensity at the back face IT is where R is the reflectance.
Transparent materials appear colored as a consequence of specific wavelength ranges of light that are
selectively absorbed; the color discerned is a result of the combination of wavelengths that are
transmitted.
10
If absorption is uniform for all visible wavelengths, the material appears colorless; examples include
high-purity inorganic glasses and high-purity and single-crystal diamonds and sapphire.
Usually, any selective absorption is by electron excitation
the fraction of the visible light having energies greater than Eg = (1.8 to 3.1 eV) is selectively
absorbed by valence bandβconduction band electron transitions.
Of course, some of this absorbed radiation is reemitted as the excited electrons drop back into their
original, lower-lying energy states. It is not necessary that this reemission occur at the same
frequency as that of the absorption. As a result, the color depends on the frequency distribution of
both transmitted and reemitted light beams.
Example: The transmissivity T of a transparent material 15 mm thick to normally incident light is
0.80. If the index of refraction of this material is 1.5, compute the thickness of material that will yield
a transmissivity of 0.70. All reflection losses should be considered.
R = (nsβ1)2 / (ns+1)2
= (1.5β1)2 / (1.5+1)2= 4.0 x 10-2
since: πΌπ = πΌ0 1 β π 2 π βπ½π
IT / I0(1βR)2=e-Ξ²l
And taking the natural logarithms of both sides of this expression gives
ln[IT / I0(1βR)2] =βΞ²l
Ξ² =β1 / l ln [IT / I0(1βR)2]
Since the transmissivity is T is equal to IT/I0, then the above equation takes the form
Ξ²=β(1/ l) ln [T / (1βR)2]
Ξ²= β(1 / 15mm) ln [0.80 / (1β4.0x10β2)2] = 9.43 x 10-3 mm-1
Colors:
β’Color determined by sum of frequencies of, transmitted light, and -re-emitted light from electron
transitions.
ο· Small differences in composition can lead to large differences in appearance
ο· β’Ex: Cadmium Sulfide (CdS)--Egap= 2.4eV,--absorbs higher energy visible light (blue,
violet),--Red/yellow/orange is transmitted and gives it color.
ο· For example, high-purity single-crystal Al2O3(sapphire) is colourless
ο· If only 0.5 - 2.0% of Cr2O3 add, the material looks red(ruby)
ο· The Cr substitutes for the Al and introduces impurity levels in the bandgap of the sapphire
ο· These levels give strong absorptions at: 400nm (green) and 600nm (blue)
leaving only red to be transmitted.
A similar technique is used to color glasses or pottery glaze by adding impurities into the molten
state:
Cu2+: blue-green, Cr3+: green
Co2+: blue-violet, Mn2+: yellow
11
β’ If Egap < 1.8eV, full absorption; color is black (Si, GaAs)
β’ If Egap > 3.1eV, no absorption; colorless (diamond)
β’ If Egap in between, partial absorption; material has a color.
ο·
ο·
reflection and absorption are dependent on wavelength and transmission is whatβs left over!
Thus the three components for a green glass are:
Example: Briefly explain why some transparent materials appear colored while others are colorless.
For a transparent material that appears colorless, any absorption within its interior is the same for all
visible wavelengths. On the other hand, if there is any selective absorption of visible light (usually by
electron excitations), the material will appear colored, its color being dependent on the frequency
distribution of the transmitted light beam.
Example: Briefly explain what determines the characteristic color of (a) a metal and (b) a
transparent nonmetal.
(a) The characteristic color of a metal is determined by the distribution of wavelengths of the
nonabsorbed light radiation that is reflected.
(b) The characteristic color of a transparent nonmetal is determined by the distribution of
wavelengths of the nonabsorbed light radiation that is transmitted through the material.
Translucency:
ο·
Even after the light has entered the material, it might yet be reflected out again due to
scattering inside the material.
ο· Even the transmitted light can lose information by being scattered internally. So a beam of
light will spread out or an image will become blurred.
ο· In extreme cases, the material could become opaque due to excessive internal scattering.
ο· Scattering can come from obvious causes:
ο grain boundaries in poly-crystalline materials
ο fine pores in ceramics
ο different phases of materials
ο· In highly pure materials, scattering still occurs and an important contribution comes from
Rayleigh scattering
ο· This is due to small, random differences in refractive index from place to place.
ο· In amorphous materials such as glass this is typically due to density or compositional
differences in the random structure.
12
ο·
ο·
ο·
ο·
In crystals, lattice defects, thermal motion of atoms etc. also give rise to Rayleigh scattering.
Rayleigh scattering also causes the sky to be blue. The reason for this is the wavelengthdependence of Rayleigh scattering:
ο scattering goes as Ξ»-4.
ο so since Ξ» red~ 2 Ξ» blue light is scattered ~16 times more than red light
This mechanism is of great technological importance because it governs losses in optical
fibers for communication.
But before we get onto fibers, we will mention a couple more basic effects
Figure: Rayleigh scattering involves the polarization of a small dielectric particle or a region that is much smaller than
the light wavelength. The field forces dipole oscillations in the particle (by polarizing it) which leads to the emission of
EM waves in "many" directions so that a portion of the light energy is directed away from the incident beam.
Figure : Photograph showing the light
transmittance of three aluminum oxide
specimens. From left to right; singlecrystal material (sapphire), which is
transparent; a polycrystalline and fully
dense (nonporous) material, which is
translucent; and a polycrystalline material
that contains approximately 5% porosity,
which is opaque.
Optical applications:
β’ Light interacts with a material in many ways.
β’ Depending on the material, its crystal-/micro-structure, and also on the characteristics of incident
light, there are many phenomena occurs, which are known as optical phenomena. These include:
o luminescence
o lasers
o thermal emission
o photo-conductivity
o optical fibers
β’ All these find quite many applications in technology for everyday life
13
Luminescence
β’ It is the process where a material absorbs energy and then immediately emits visible or near-visible
radiation. It consists of electron excitation and then dropping down to lower energy states. Visible
light is emitted when it falls back to a lower energy state if 1.8 eV < βπ < 3.1 eV.
-8
β’ If the reemission of radiation occurs within 10 sec after excitation, the luminescence is called
-8
fluorescence, and if it takes longer than 10 sec, it is known as phosphorescence.
β’ Special materials called phosphors have the capability of absorbing high-energy radiation and
spontaneously emitting lower-energy radiation. Ex.: some sulfides, oxides, tungstates, and few
organic materials. Ordinarily, pure materials do not display these phenomena, and to induce them,
impurities in controlled concentrations must be added.
β’ The intensity of luminescence is given as: πΌ = πΌ0 exp β
π‘
π
β’ where I β initial intensity of luminescence,
0
ο I β fraction of luminescence after time, t,
ο Ο - relaxation time, constant for a material.
β’ Luminescence process is classified based on the energy source for electron excitation as photoluminescence, cathode-luminescence, and electro-luminescence.
Photo-luminescence
β’ Photo-luminescence occurs in fluorescent lamps. Arc between electrodes excites mercury in lamp
to higher energy level. Electron falls back emitting UV light . Fluorescent lamps consist of a glass
housing, coated on the inside with specially prepared tungstates or silicates. Ultraviolet light is
generated within the tube from a mercury glow discharge, which causes the coating to fluoresce and
emit white light.
β’ Here ultra-violet radiation from low-pressure mercury arc is converted to visible light by calcium
halo-phosphate phosphor (Ca F P O ).
10 2 6
24
-
-
β’ In commercial lamps, about 20% of F ions are replaced with Cl ions.
3+
2+
β’ Antimony, Sb , ions provide a blue emission while manganese, Mn , ions provide an orange-red
emission band.
Cathode-luminescence:
β’ Cathode-luminescence is produced by an energized cathode which generates a beam of highenergy bombarding electrons.
β’ Applications of this include electron microscope; cathode-ray oscilloscope; color television
screens.
β’ The modern televisions have very narrow, about 0.25 mm wide, vertical stripes of red-, green-, and
blue- emitting phosphors deposited on the inner surface of the screens.
β’ Commercial phosphors for different colors are: red β yttrium oxy-sulfide (Y O S) with 3%
+
3+
2
2
europium (Eu); green β (Zn,Cd)S with a Cu acceptor and Al donor; blue β zinc sulfide (ZnS)
+
-
with Ag acceptor and Cl donor.
14
Electro-luminescence:
β’ Electro-luminescence occurs in devices with p-n rectifying junctions which are stimulated by an
externally applied voltage.
β’ When a forward biased voltage is applied across the device, electrons and holes recombine at the
junction and emit photons in the visible range (mono-chromatic light i.e. singe color). These
diodes are called light emitting diodes (LEDs).
β’ LEDs emit light of many colors, from red to violet, depending on the composition of the
semiconductor material used.
β’ Ex.: GaAs, GaP, GaAlAs, and GaAsP are typical materials for LEDs.
β’ Materials for colored LEDs are
Wave length (nm)
Color
Material
-
Infra-red
GaAs
660
Red
GaP
Al
0.40
0.25
GaP
As
0.60
Ga
0.75
or
As
635
Orange
578
Yellow
GaP0.85As0.15
556
Green
GaP
(GaP1.00As0.00)
-
Blue
Ga0.94NIn0.06
0.65
As
0.35
Lasers :
β’ Laser is an acronym for light amplification by
stimulated emission of radiation. It is in fact special
application of luminescence.
β’ Unlike most radiation processes, such as luminescence,
which produce incoherent light, the light produced by
laser emission is coherent.
β’ All of the light emission we have mentioned so far is
spontaneous. It happened just due to randomly
occurring βnaturalβ effects
β’ Stimulated emission refers to electron transitions that are βencouragedβ by the presence of other
photons
β’ Einstein showed that an incident photon with E β₯Eg was equally likely to cause stimulated
emission of light as to be absorbed
β’ The emitted light has the same energy and phase as the incident light (= coherent)
15
β’ Under normal circumstances, there are few excited electrons and many in the ground-state,
so we get predominantly absorption.
β’ If we could arrange for more excited than non-excited electrons, then we would get mostly
stimulated emission.
β’ This is based on the fact that in certain materials, electrons excited by a stimulus produce photons
which in turn excite additional photons of identical wavelength. Thus a large amplification of the
photons emitted in the material occurs, as shown in figure below.
β’ Lasers are useful in many applications such as welding, metal cutting, heat treatment, surgery,
mapping, reading compact disks, etc. Ex.: Ruby, single crystal of Al O doped with little amount
2
3
of Cr O ; yttrium aluminium garnet (Y Al O β YAG) doped with neodymium, Nd; CO gas;
2
3
3
5
12
2
He-Ne gas; some semi-conductors like GaAs and InGaAsP.
Presented in this figure is an illustration of the
gain, or amplification, that occurs with
increased path length in the resonant cavity
due to the mirrors at each end. Figure (a)
shows the beginning of stimulated
emission, which is amplified in figure (b)
through Figure (g) as the light is reflected
from the mirrors positioned at the cavity
ends. A portion of light passes through the
partially reflected mirror on the right-hand
side of the cavity (figures (b,d, and f))
during each pass. Finally, at the equilibrium
state (figure (h)), the cavity is saturated
with stimulated emission.
16
Thermal emission
β’ When a material is heated, electrons are excited to
higher energy levels, particularly in the outer
energy levels where the electrons are less
strongly bound to the nucleus.
β’ These excited electrons, upon dropping back to the
ground state, release photons in process what is
called thermal emission.
β’ During thermal emission a continuous spectrum of
radiation is emitted with a minimum wavelength
and the intensity distribution is dependent on the
temperature as shown in figure beside.
β’ Higher the temperature, wider will be the range of
wavelengths emitted. By measuring the intensity
of a narrow band of the emitted wavelengths
with a pyrometer, materialβs temperature can be estimated.
Photo-conductivity
ο·
The conductivity of semiconducting materials depends on the number of free electrons in the
conduction band and also the number of holes in the valence band
β’ Bombardment of semiconductors by photons, with energy equal to greater than the band gap, may
result in creation of electron-hole pairs that can be used to generate current. This process is called
photo-conductivity.
β’ It is different from photo-electric effect in the sense that an electron-hole pair is generated whose energy
is related to the band gap energy instead of free electron alone whose energy is related to the Fermi
level.
β’ The current produced in photo-conductivity is directly related to the incident light intensity.
β’ This phenomenon is utilized in photographic light meters. Cadmium sulfide (CdS) is commonly used
for the detection of visible light, as in light meters.
β’ Photo-conductivity is also the underlying principle of the photo-voltaic cell, known to common man as
solar cell, used for conversion of solar energy (sunlight) into electricity.
17
Optical fibers :
β’ Optical fibers have revolutionized the communication industry.
β’ These systems consists of transmitter (a semiconductor laser) to
convert electrical signals to light signals, optical fiber to
transmit the light signals, and a photodiode to convert light
signals back to electrical signals.
β’ It primarily consists of core, cladding and coating. The core
transmits the signals, while the cladding constrains the light
beam to the core; outer coating protects the core and cladding
from the external environment.
β’ Typically both the core and cladding are made of special types
of glass with carefully controlled indices of refraction.
β’ The indices of refraction are selected such that
πππππππππ < ππππ
β’ Once the light enters the core from the source, it is reflected
internally and propagates along the length of the fiber.
β’ Internal reflection is accomplished by varying the index of
refraction of the core and cladding glass materials. Usually
two designs are employed in this regard.
Types of optical fibers
β’ In step-index optical fiber, there is a sharp change in refractive
index between the core and cladding. In this design output
pulse will be broader than the input one. It is because light rays
traveling in different trajectories have a variety of path lengths.
fiber. This results in a helical path for the light rays, as opposed to zig-zag path in a step-index fiber.
β’ Here impurities such as boron oxide (B O ) or germanium dioxide (GeO ) are added to the silica glass
2
3
2
such that the index of refraction varied gradually in parabolic manner across the cross section. This
enables light to travel faster while close to the periphery than at the center. This avoids pulse
β’ Both step- and graded- index fibers are termed as multi-mode fibers.
β’ Third type optical fiber is called single-mode fiber in which light travels largely parallel to the fiber axis
with little distortion of the digital light pulse. These are used for long transmission lines.
18
Optical fiber properties
β’ Core and cladding materials are selected not only on the basis of their refractive indices, but also on
basis of ease of manufacturability, light loss, mechanical strength properties and dispersion
properties.
β’ However, density (Ο) and refractive index (n) are critical. These two parameters are related
approximately as
π + 10.4
8.6
β’ High-purity silica-based glasses are used as fiber material, with fiber diameter ranging from 5 to 100
ΞΌm.
π=
β’ The fibers are carefully fabricated to be virtually free from flaws
19
Example: The intensity of light absorbed while passing through a 16-kilometer length of optical
fiber glass is equivalent to the light intensity absorbed through for a 25-mm thickness of ordinary
window glass. Calculate the absorption coefficient Ξ² of the optical fiber glass if the value of b for the
window glass is 10-4 mm-1.
π°β²π» = π°β²π πβπ·π ,
π°β²π»
π°β²π
= πβ
ππβπ ππβπ ππ.πππ
= π. ππππ
Ξ² =(β1 / x) ln ( IT' / I0')
Now, solving for Ξ² leads to
Ξ²=β(1 / x) ln (IT'I0')
For x = 16 km = 16 x 103 m = 16 x 106 mm
Ξ²=β (1 / 16x106mm) ln(0.9975)=1.56x10β10mmβ1
20
```
Related documents